# Statistical methods applied for materials selection

Statistical methods applied for materials selection
C. Târcolea, A. Paris, A. Demetrescu-Târcolea
Abstract. In the design process the choice of materials for a new product
is made from a very large spectrum. Usually in the first stage, for each
material, it is taken into consideration, as many attributes as possible
is. In the second stage it is taken into consideration only a few ”virtual”
attributes (usually two or three), given by principal component analysis.
The main idea is exemplified by the particular case of fiberglass-reinforced
thermoplastics.
M.S.C. 2000: 62H25, 62J15.
Key words: Principal component analysis, artificial factors.
1
Introduction
”The goal of design is create products that perform their function effectively, safely,
at acceptable cost” (Ashby, 1999) [1]. The choice of a material for a product is not
based on all the attributes, is based on a combination of properties. In this paper it is
presented a method of reduction of attributes to a combination of a few artificial factors. The selection of the materials group uses the following premises: -the taking into
consideration of an ever larger spectrum of materials, otherwise expressed, defining
as complete as possible the selection range -the division of materials in ”equivalence
classes” otherwise expressed as the classification of materials thus obtaining a significant reduction of the selection space, the initial chaotically multitude is reduced
to smaller number of classes, the number of each class having common properties,
processes accompanied or not by the elimination or some materials taken into consideration - the establishing of the same simple and efficient methods of selection, with
the possibility of implementing on a computer [1], [2], [8].
A possibility of getting down the properties range is the taking into consideration
of the correlation between the properties, studying thus only a few independent properties to the possible extent. The introduction of the up-to-date calculation enables
the data stocking concerning the properties, from the standard version, under the
normal temperature and the time t = 0, up to more complete versions, taking into
account their variability as against the temperature, time, etc.[8].
The classification of materials is often empirically made, for example in six groups
[2,8] metallically materials, polymers, elastomers, glasses, ceramics and compound
Applied Sciences, Vol.11, 2009, pp.
145-150.
c Balkan Society of Geometers, Geometry Balkan Press 2009.
&deg;
146
C. Târcolea, A. Paris, A. Demetrescu-Târcolea
materials. Another variant [8] uses as criterion the cristallinity of materials (crystalline or non-crystalline and compound) each class being grouped in underclasses as
per the structure type, way of obtaining, etc.
2
Application of principal component analysis
The PCA is a standard technique to reduce multivariate data sets in a subspace
of small dimension, in our case a trivariate one [3,10]. The number of observable
attributes gives the dimension of the initial representation space of the objects [6,7].
Instead of realer attributes, the PCA uses new factors, but artificial ones. In the
present paper, the dimensional reduction of attributes for a family of materials follows
the Jöreskog’s researches [4,5].
Let only 9 materials (objects), each of them having 6 attributes (table 1). The
resulted three-dimensional subspace gives a minimal deformation of distances through
projection. As illustration let’s take an application from ”Reinforced Plastics Handbook” p. 889 [9], concerning selecting plastics and process: for nine glass fiber
(30wt%) reinforced thermoplastics are presented six important mechanical and cost
properties for a detailed analysis.
Prop. / Materials
ABS
P1
1.29
POM(c.c.)
1.63
ETFE
1.89
PA 6
1.37
6/6
1.38
6/6(f.r.)
1.59
6/10, 6/12
1.30
PPA
1.43
LCP
1.57
P2
100
(14.5)
134
(19.5)
97
(14)
159
(23)
179
(26)
134
(19.5)
148
(21.5)
221
(32)
162
(23.5)
P3
7.58
(1100)
9.65
(1400)
7.24
(1050)
8.27
(1200)
8.96
(1300)
7.58
(1100)
7.58
(1100)
11.4
(1650)
12.8
(3120)
P4
102
(215)
166
(330)
238
(460)
216
(120)
254
(490)
243
(470)
214
(117)
285
(545)
318
(614)
P5
69
(1.3)
96
(1.8)
320
(6)
123
(2.3)
107
(2)
69
(1.3)
128
(2.1)
118
(2.2)
85
(1.7)
Table 1. Analyzed properties of nine thermoplastics
The matrix X is a 6 &times; 9 dimensional matrix, attributes/materials:
P6
1.4
2.2
19
1.9
2.7
(3.3)
1
6.2
32
Statistical methods applied for materials selection







X=






1, 29 100 7, 58 102
1, 63 134 9, 65 166
1, 89 97 7, 24 238
1, 37 159 8, 27 216
1, 38 179 8, 96 254
1, 59 134 758 243
1, 3 148 7, 58 214
1, 43 221 11, 4 285
1, 57 162 12, 8 318
147

69 1, 4
96 2, 2 

320 19 

123 1, 9 

107 2, 7 

69 3, 3 

128
1 

118 6, 2 
85 32
The standardized matrix of X, denoted Z, is:







Z=






−1, 0522
−1, 25
0, 69766 −0, 369
2, 03579 −1, 328
−0, 6405 0, 2794
−0, 589 0, 7979
0, 49179 −0, 369
−1, 0007 −0, 006
−0, 3317 1, 8867
0, 38886 0, 3572
−0, 3398 −1, 953
−0, 3315 −0, 947
−0, 3411
0, 185
−0, 337 −0, 161
−0, 3342
0, 437
2, 66659
0, 264
−0, 3398 −0, 192
−0, 3245
0, 924
−0, 3188
1, 443
Based on matrix equation
R=
it results that:




R=



−0, 715
−0, 363
2, 5555
−0, 012
−0, 22
−0, 715
0, 0536
−0, 077
−0, 507
−0, 5938
−0, 5189
1, 05346
−0, 547
−0, 4721
−0, 416
−0, 6312
−0, 1446
2, 2702














1
Ztr ∗ Z,
8
1 −0, 36956 0, 184942
−0, 3696
1 −0, 13352
0, 18494 −0, 13352
1
0, 27414
0, 62622 0, 103873
0, 6577 −0, 32582 −0, 27123
0, 54921 −0, 03745
−0, 1519
(1)

0, 274144 0, 657701 0, 549213
0, 626218 −0, 32582 −0, 03745 

0, 103873 −0, 27123 −0, 1519 

1 0, 139821 0, 610039 

0, 139821
1 0, 317506 
0, 610039 0, 317506
1
It is obvious that R is the correlation matrix. The proximity between attributes is
expressed in terms of correlations. The inverse matrix of R is:


4, 24886 −2, 28953 −3, 00663 3, 409168 −3, 62451 −3, 80489
 −2, 2895
16, 1683 8, 535721 −18, 9344 7, 857795 12, 21537 



−3, 0066
8, 53572
6, 48209 −10, 6674 5, 564535 7, 696317 
−1


R =

 3, 40917 −18, 9344 −10, 6674 24, 00877 −9, 64994 −15, 7842 
 −3, 6245
7, 8578 5, 564535 −9, 64994 6, 605492 6, 919718 
−3, 8049
12, 2154 7, 696317 −15, 7842 6, 919718 12, 14818
It obtains: diag(R−1 ) = diag(4.2488; 16.168; 6.482; 24.008; 6.605; 12.148)
1
diag(R−1 ) 2 = diag(2.061; 4.021; 2.546; 4.899; 2.570; 3.485)
diag(R−1 )−1 = diag(0.235; 0.0618; 0.154; 0.0416; 0.151; 0.082).
148
C. Târcolea, A. Paris, A. Demetrescu-Târcolea
Jöreskog’s method considers that theoretical covariance matrix of the standardized
attributes, V , is factorized as:
V = Ltr ∗ L + diag(s21 , . . . , s26 ).
(2)
For the uniqueness of the estimators of the matrices from the decomposition of V it
is supposed that the variances are direct proportional with the inverse values of the
diagonal elements of the matrix V −1 ; that is:
diag(s21 , . . . , s26 ) = m(diag(V −1 ))−1 ,
(3)
where m is the proportional parameter. Further on, it is denoted by R∗ the following
matrix:
1
1
R∗ = diag(R−1 )) 2 ∗ R ∗ diag(R−1 )) 2
(4)
It results:




R∗ = 



4, 248862 −3, 06309
−3, 06309 16, 16834
0, 970577 −1, 3669
2, 768855 12, 33796
3, 484313 −3, 36711
3, 945777 −0, 52491
0, 970577
−1, 3669
6, 48209
1, 295822
−1, 77477
−1, 34791

2, 768855 3, 484313 3, 945777
12, 33796 −3, 36711 −0, 52491 

1, 295822 −1, 77477 −1, 34791 
.
24, 00877 1, 760794 10, 41833 

1, 760794 6, 605492 2, 844202 
10, 41833 2, 844202 12, 14818
The eigenvalues of this matrix are given in the table 2 and the first three eigenvectors
in the table 3:
36,14978
19,16469
8,017578
5,002533
1,114291
0,212852
Table 2. Eigenvalues of the matrix R∗
Because
λ1 + λ2 + λ3
≈ 0.91 &gt; 0.90
λ1 + λ2 + λ3 + λ4 + λ5 + λ6
it can be considered only the 3-dimensional subspace.
T
−0, 0726
−0, 46987
0, 002525
−0, 80398
−0, 03727
−0, 3552
U
0, 379876
−0, 62708
−0, 01
0, 075068
0, 407536
0, 53912
W
−0, 13195
0, 215822
−0, 89147
−0, 18658
0, 301071
0, 125862
Table 3. The values of the first three eigenvectors of the matrix R∗
An estimator for the parameter m is the average of the remained eigenvalues:
m=
1
(λ4 + λ5 + λ6 ) = 2.11
3
The parameters of interest are the variances, given by:
s2i =
m
,
rii
i ∈ 1, 6
(5)
Statistical methods applied for materials selection
149
where rii is the element ii of the matrix R−1 .
In the present case, it is obtained the values of s2i (table 4):
0, 49660356 0, 130502 0, 325512
0, 087885 0, 319431
0, 173689
Table 4. Values of s2i
Further on, it should be calculate:
ki2 = 1 − s2i ,
i = 1, 6
(6)
The results are given in the table 5:
0, 50339644 0, 869498 0, 674488
0, 912115 0, 680569
0, 826311
Table 5. Values of ki2
The three eigenvectors, denoted as T, U, W associated with the first three chosen
eigenvalues are determined so that:
||T ||2 = λ1 − m̂,
||U ||2 = λ2 − m̂,
||W ||2 = λ3 − m̂.
(7)
The matrix of these eigenvectors is:


−0, 42355 1, 568786 −0, 32071
 −2, 74139 −2, 58965 0, 524566 


 0, 014732
−0, 0413 −2, 16675 

A=
 −4, 69073 0, 310011
−0, 4535 


 −0, 21747 1, 683015 0, 731768 
−2, 07237 2, 226422 0, 305914
1
L = (diag(R−1 ))− 2 ∗ A,




L=



It results:
−0, 20548
−0, 68177
0, 005786
−0, 95732
−0, 08461
−0, 59458
0, 761075
−0, 64403
−0, 01622
0, 063269
0, 65484
0, 638781
2
2
ki2 ∼
+ li2
+ L2i3 ,
= li1
−0, 15559
0, 130457
−0, 85104
−0, 09255
0, 284722
0, 08777
for i ∈ 1, 6,
(8)








(9)
which confirm the correctness of the model.
3
Conclusions
Revising the up-to-date problems of the materials selection, it was emphasized on the
statistical approach, starting from the bi-or three dimensional graphical drawing of
some properties. The design engineer should have in this manner at his disposal an
effective system, optimum for the selection of the material. The ellipse or ellipsoid
150
C. Târcolea, A. Paris, A. Demetrescu-Târcolea
may be built, as in the shown method, all the possibility of assuming some different
probabilities for the random vector to take the values in the area bounded by the
ellipse or ellipsoid.
The application of this model will simplifies the materials design and there are
many other possible extensions in the design process. Furthermore, a mixture between
Jöreskog’ method and materials design principles is useful for the developments.
References
[1] M. F. Ashby, Materials selection in mechanical design. Butterworth-Heinemann
Edition, Oxford GB, 1999.
[2] M. F. Ashby, K. Johnson, Materials and Design, the Art and Science of Materials
Selection in Product Design, Butterworth Heinemann, Oxford, GB, 2002.
[3] M. Dumitrescu, A. Batatorescu, Applied Statistics using the R-System, Editura
Universitatii din Bucuresti, 2006.
[4] J. Hartung, B.Elpelt, Multivariate Statistik, Oldenbourg Verlag, München, Germany 1986.
[5] K. G. Jöreskog, Statistical Estimation in Factor Analysis, a New Technique and
Its Foundations, Ed. Almquist&amp;Wiksell, Uppsala, 1963.
[6] L. Lemnete-Ninulescu, A moment problem with values positive definite matrices,
BSG PROCEEDINGS 14, (MENP-4), 2006, Bucharest, ROMANIA, Geometry
Balkan Press (2007), 95-98.
[7] M. Migdalovici, D. Baran, Theoretical research the Floquet stability theorem with
applications, BSG (MENP-4), 2006, Bucharest, ROMANIA, Geometry Balkan
Press (2007), 106-110.
[8] A. Paris, S. Ionescu, P. Szel, C. Târcolea, Statistical approach in the selection
of materials for engineering products. Scientific Seminar ”Modern mechanical
design” Bucharest, U.P.B. (1991), 97-106.
[9] D. V. Rosato, Reinforced Plastics Handbook, Elsevier Edition, B.V. 2005.
[10] C. Târcolea, A. Paris, The Jöreskog technique applied for materials design, Proceedings of the 17-th, ICMaS, Ed Acad. Romane, (2008), 309-312.